- Erosion corrosion of copper water tubes
Erosion corrosion, also known as impingement damage, is the combined effect of
corrosionand erosioncaused by rapid flowing turbulent water. It is probably the second most common cause of copper tube failures behind Type 1 pitting which is also known as Cold Water Pitting of Copper Tube.
Copper water tubes
Coppertubes have been used to distribute potable water within building for many years and hundreds of miles are installed throughout Europeevery year. The long life of copper when exposed to natural waters is a result of its thermodynamicstability, its high resistance to reacting with the environment, and the formation of insoluble corrosion products that insulate the metal from the environment. The corrosion rate of copper in most potable waters is less than 25 µm/year, at this rate a 15 mm tube with a wall thickness of 0.7 mm would last for about 28 years. In some soft waters the general corrosion rate may increase to 125 µm/year, but even at this rate it would take over 5 years to perforate the same tube.
If the general water speed or the degree of local turbulence in an installation is high, the protective film that would normally be formed on a copper tube as a result of slight initial corrosion, may be torn off the surface locally, permitting further corrosion to take place at that point. If this process continues it can produce deep localised attack of the type known as erosion-corrosion or impingement damage. The actual attack on the metal is by the corrosive action of the water to which it is exposed while the erosive factor is the mechanical removal of the corrosion product from the surface.
Impingement attack produces highly characteristic water-swept pits, which are often horseshoe shaped, or it can produce broader areas of attack. The leading edge of the pit is frequently undercut by the swirling action of the water. Usually, the surface of the metal within the pits or areas of attack is smooth and carries no substantial corrosion product. Corrosion-erosion is known to occur in pumped-circulation hot water distribution systems, and even in cold water distribution systems, if the water velocities are too high. The factors influencing the attack include the chemical character of the water passing through the system, the temperature, the average water velocity in the system and the presence of any local features likely to induce turbulence in the water stream.
It is unusual for the general water velocity in a system to be so high that impingement attack occurs throughout the whole of the copper pipework. More commonly, the velocity is just sufficiently low for satisfactory protective films to be formed and to remain in position on most of the system, with impingement damage more likely to occur where there is an abrupt change in the direction of water flow giving rise to a high degree of turbulence, such as at tee pieces and elbow fittings. It is not generally realised how great an effect small obstructions can have on the flow pattern of water in a pipe-work system and the extent to which they can induce turbulence and cause corrosion-erosion. For example, it is most important, as far as possible, to ensure that copper tubes cut with a tube cutter are deburred before making the joint. Also a gap between the tube end and the stop in the fitting, due to the tube not having been cut to the correct length and fully inserted into the socket of the fitting, can also induce turbulence in the water stream.
The rate of impingement attack on copper also depends to some extent on the temperature of the water. The maximum velocities for fresh waters at different temperatures recommended in
Swedenare given in the table below. These figures are for aerated waters of pHnot less than about 7.
Recommended Maximum Water Velocities at Different Temperatures for Copper (m/s)
§ These velocities give a risk of impingement attack and are acceptable only for small bore connections to taps, flushing cisterns etc., through which water flow is intermittent.
BS 6700 gives the following maximum water velocities although it does note that these are currently under investigation and the velocities specified will be amended if the results of this investigation so require.
The minimum water speed at which copper pipes suffer impingement attack depends also to some extent on water composition. Aggressive waters that tend to be cupro-solvent are the most likely to give rise to impingement attack. Installations in large buildings where flow rates may be high and water is in continuous circulation are much more susceptible to attack than ordinary domestic installations. A high mineral content or a pH below 7 is likely to increase the possibility of corrosion-erosion occurring while a positive Langelier Index and consequent tendency to deposit a calcium carbonate scale is generally beneficial. The presence or absence of colloidal organic matter is also probably of some importance.
Remedial measures for impingement attack include modifications to the system to reduce the average water velocity, e.g. by using larger diameter tubes or, if appropriate, to lower the pump speed, and/or to redesign the part of the installation concerned to eliminate the cause of local turbulence, e.g. by using slow or swept bends and tee fittings rather than elbows and square tees. It is important to minimise the possibility of any local turbulence occurring by ensuring that the ends of tubes cut with a tube cutter are deburred and that the tubes are inserted fully to the stops in the fitting before the joints are made, as referred to earlier in this section. In some cases, where the above approaches are not possible, the length of copper tube affected can sometimes be replaced by materials more resistant to corrosion-erosion, e.g. 90/10 copper-nickel (BS Designation CN102) using appropriate fittings, or stainless steel to BS 4127:1994.
* [http://www.corrosionlab.com/papers/erosion-corrosion/erosion-corrosion.htm Erosion Corrosion] from Corrosion Testing Laboratories, Inc.
* [http://www.corrosionist.com/copper_pipe_corrosion.htm Copper pipe Corrosion] Copper pipe Corrosion theory and mechanims
Wikimedia Foundation. 2010.
Look at other dictionaries:
Copper — For other uses, see Copper (disambiguation) … Wikipedia
Water heating — is a thermodynamic process using an energy source to heat water above its initial temperature. Typical domestic uses of hot water are for cooking, cleaning, bathing, and space heating. In industry, both hot water and water heated to steam have… … Wikipedia
Cold water pitting of copper tube — occurs in only a minority of installations. Copper water tubes are usually guaranteed by the manufacturer against manufacturing defects for a period of 50 years. The vast majority of copper systems far exceed this time period but a small minority … Wikipedia
Flow-accelerated corrosion — (FAC), also known as flow assisted corrosion, is a corrosion mechanism in which a normally protective oxide layer on a metal surface dissolves in a fast flowing water. The underlying metal corrodes to re create the oxide, and thus the metal loss… … Wikipedia
Tap water — Indoor Tap commonly found in the bathroom or kitchen. This tap is a single handle, double spout tap (one spout for hot water, one spout for cold water). Tap water (running water, city water, municipal water, etc.) is a principal component of… … Wikipedia
Cavitation — is defined as the phenomenon of formation of vapour bubbles of a flowing liquid in a region where the pressure of the liquid falls below its vapour pressure. Cavitation is usually divided into two classes of behavior: inertial (or transient)… … Wikipedia
Surface condenser — A surface condenser is a commonly used term for a water cooled shell and tube heat exchanger installed on the exhaust steam from a steam turbine in thermal power stations. These condensers are heat exchangers which convert steam from its … Wikipedia
Fouling — This article is about fouling in engineering. For uses of the term foul outside technology, see Foul (disambiguation). Not to be confused with fowling. Heat exchanger in a steam power plant, fouled by macro fouling … Wikipedia
nickel processing — Introduction preparation of the metal for use in various products. Although it is best known for its use in coinage, nickel (Ni) has become much more important for its many industrial applications, which owe their importance to a… … Universalium
tunnels and underground excavations — ▪ engineering Introduction Great tunnels of the world Great tunnels of the worldhorizontal underground passageway produced by excavation or occasionally by nature s action in dissolving a soluble rock, such as limestone. A vertical opening … Universalium